Shortening crack mitigation crack evaluation TN451-010616 ... Q.6.1. Crack Evaluation Q.6.2. Cracks
Embed Size (px)
Transcript of Shortening crack mitigation crack evaluation TN451-010616 ... Q.6.1. Crack Evaluation Q.6.2. Cracks
Post-Tensioning Expertise and Design Technical Note 451 January 2016
CRACK MITIGATION AND EVALUATION1
Shortening of Post-Tensioned Members and Restraint of Supports
Bijan O Aalami2
CONTENTS Q.1 OVERVIEW Q.2 COMPUTATION OF SHORTENING
Q.2.2 Shortening from Shrinkage Q.2.3 Shortening from Creep Q.2.4 Elastic Shortening Q.2.5 Temperature Effects Q.2.6 Shortening Example Q.2.7 Estimate of Short-Term Shortening Q.2.8 Short-Term Shortening Example
Q.3 MITIGATION OF RESTRAINT CRACKS Q.3.1 Assumptions and Overview Q.3.2 Characteristics of Restraint Cracks Q.3.3 Crack Mitigation Options;
Q.3.3.1 Favorable Layout Q.3.3.2 Structural Separation Q.3.3.3 Delay (Closure) Strips; Joints; Favorable Pour Sequence Q.3.3.4 Permanent Released Connections Q.3.3.5 Other Released Connections Q.3.3.6 Detailing
Q.4 CRACK MITIGATION EXAMPLES Q.4.1 Podium Slab on Perimeter Walls Q.4.2 Example of a Multistory Building
R.1 IMPACT OF SUPPORT RESTRAINT ON FLOOR SAFETY R.1.1 Restraint Cracks and Safety R.1.2 Unbonded Tendons; Safety and Restraint Cracks R.1.3 Bonded Tendons; Safety and Restraint Cracks
R.2 COMPARISON BETWEEN UNBONDED AND BONDED SYSTEMS
1 Copyright Bijan O. Aalami, 2015; bijan@PT-Structures.com; www.PT-Structures.com 2 Professor Emeritus, San Francisco State University; Principal, ADAPT Corporation; www.adaptsoft.com
mailto:bijan@PT-Structures.com; http://www.PT-Structures.com http://www.adaptsoft.com
TN451 - 2
Q.6 REPAIR OF RESTRAINT CRACKS Q.6.1. Crack Evaluation Q.6.2. Cracks to Repair Q.6.3. Time of Repair Q.6.4. Method of Repair
Q.7 REFERENCES Q.8 NOTATIONS
Q.1 OVERVIEW In post-tensioned construction, the tendons are stressed and anchored after the concrete member they are embedded in has developed sufficient strength (Fig. Q.1-1a). The tension in the tendons results in an equivalent compression in the concrete, which causes the member to shorten (Fig. Q.1-1b). In most applications, the tendons are profiled so that they also exert a vertical force on the member (Fig. Q.1-1c). the vertical force results in a bending moment in the member; the tendon profile is usually selected to counteract the bending of the member under selfweight, thus reducing the bending under normal loading. This Technical Note deals with the shortening of a post-tensioned member caused by the precompression; the possible restraint of the member’s supports to shortening; the possibility of crack formation in the member from this restraint; and finally the evaluation of restraint cracks.
FIGURE Q.1-1 Basics of Post-Tensioning Construction
Because concrete is not a completely rigid material, the post-tensioning force P will compress a free-standing concrete member, and shorten it. The compressive stress f resulting in the member from the application of the force P leads to the member’s shortening u. The relationship between the compressive stress in the member and its shortening is governed by the material properties of the member and is generally similar to Fig. Q.1-2a . .
TN451 - 3
FIGURE Q.1-2 Precompression and Shortening
In actual construction, post-tensioned members such as floor slabs and beams are supported on walls and columns. These supports can restrain the free shortening of the member when the tendons are stressed. Unless the member is allowed to shorten, as shown in Fig. Q.1-3, it will not receive the full amount of precompression from the stressed tendons. In theory, if the supports prevent any shortening (part b of the figure), the entire post-tensioning force will be diverted to the supports, leaving the member with no precompression. Failure to account for restraint from the supports can lead to cracking. Apart from possible aesthetic objections, these restraint cracks can cause leakage, and expose the reinforcement to the corrosive elements. More importantly, restraint cracks can reduce the contribution of the post-tensioning tendons to the strength capacity of the member. The extent of the restraint cracking in a post-tensioned member depends on a number of factors, including the stiffness of the supports. Figure Q.1-4 illustrates two extremes. In part (a) a post-tensioned member on very flexible supports shortens under the precompression, forcing the supports to follow the member’s moment. This can result in cracking of the supports. At the other extreme, a member on very stiff supports will be restrained against in-plane shortening and can develop restraint cracks as it shortens (part b of the figure).
TN451 - 4
FIGURE Q.1-3 Restrained and Unrestrained Members
FIGURE Q.1.4 Effects of Support Restraint on Member Cracking
Cracking due to restraint from the supports is generally most pronounced at the first level of a structure, due to the restraint from the foundation; there is less cracking at higher levels. Experienced design engineers are aware of the possibility of restraint cracking and its consequences; they use a number of measures to allow the post-tensioned member to shorten, while minimizing the effects of cracking in either the member or its supports. The first step in designing for shortening and restraint cracking of a post-tensioned member is to either calculate or estimate the anticipated long-term shortening. Section Q.2 outlines a computational procedure to determine the long-term shortening of a post-tensioned member. Section Q.3 discusses the details commonly used to reduce the potential for restraint cracking. Section Q.4 provides a guideline to estimate shortening for preliminary design and goes through two examples that illustrate the practical aspects of design for crack mitigation. Section Q.5 describes the consequences of restraint cracks on the safety of a post-tensioned member and highlights the significance of the type of post-tensioning (bonded or unbonded).
TN451 - 5
Q.2 COMPUTATION OF SHORTENING The long-term shortening of a post-tensioned member is primarily the result of: v Shrinkage; v Creep; v Elastic shortening; and v Temperature change. Much is available in the literature on the contribution of each of the above parameters and the interactions among them. Most of the literature on shortening of concrete members is based on test specimens observed in the controlled environment of research laboratories. The environment of an actual structure will not match that of these test specimens, however. While it is possible to estimate shortening by taking a test specimen from the concrete of the actual structure and curing it in the same environment as the structure, this is not often done. Testing would provide useful data for other structures under the same conditions but would not help with design of the structure being tested. The typical practice is to start with the base values observed in the laboratory specimen and adjust them to reflect the conditions of the actual structure. The adjustment is done by applying various correction factors, each of which accounts for one of the variations between the environment of the actual structure and the environment of the standard test specimen. Much is available in the literature on the contribution of each of the above parameters and the interactions among them. Most of the literature on shortening of concrete members is based on test specimens observed in the controlled environment of research laboratories. The environment of an actual structure will not match that of these test specimens, however. While it is possible to estimate shortening by taking a test specimen from the concrete of the actual structure and curing it in the same environment as the structure, this is not often done. Testing would provide useful data for other structures under the same conditions but would not help with design of the structure being tested. The typical practice is to start with the base values observed in the laboratory specimen and adjust them to reflect the conditions of the actual structure. The adjustment is done by applying various correction factors, each of which accounts for one of the variations between the environment of the actual structure and the environment of the standard test specimen. v The effects of each of the shortening components are independent from one another and can be estimated on their
own. v The parameters of the structure are within the applicable range of the suggested correction factors. These are: § Concrete weight: W= 140 – 155 pcf (2300 - 2600 kg/m3) § Concrete strength (28 day cylinder): f’c = 3000 to 6000 psi ( 21 to 40 MPa ) § Average precompression: P/A = 100 to 350 psi (0.8 to 2.40 MPa )
The total shortening of a post-tensioned member meeting the above criteria can be expressed as follows: a= L ( ES + SH + CR + TEM ) (Exp Q.2-1) Where, a = total shortening; CR = creep shortening strain;
TN451 - 6
ES = elastic shortening strain; L = length of the member; and SH = shrinkage shortening strain; and TEM = strain due to drop in temperature.
The creep and shrinkage values obtained through laboratory tests are referred to as the “base shrinkage strain” SHo and
“base creep coefficient” CRo. S